- Nano Express
- Open Access
Solution-Processed Inorganic Perovskite Flexible Photodetectors with High Performance
Nanoscale Research Letters volume 14, Article number: 284 (2019)
All inorganic CsPbI3-xBrx perovskites have been widely used in photodetectors due to their excellent optoelectronic properties and simple preparation processes. Here, high-performance flexible photodetectors based on inorganic CsPbI3-xBrx perovskites are demonstrated, which are achieved by a modified solution-processed method. When biased at a low voltage of 10 mV, the device yielded fast response speeds (90 μs /110 μs for CsPbI2Br PDs and 100 μs/140 μs for CsPbIBr2 PDs), a high on/off ratio of 104, and a high detectivity about 1012 Jones. Meanwhile, the devices showed outstanding environmental stability and mechanical flexibility. The periodic I-t curves had negligible fluctuation (< 5%) after storing in air atmosphere for 30 days or bending for 100 times. The results indicate that CsPbI3-xBrx perovskites have great potential in photodetection areas and pave the way to achieve high-performance flexible PDs.
In the past few decades, a variety of inorganic semiconductor materials have drawn most attention of photodetectors research, such as InGaAs, GaN, ZnO, and Si [1,2,3,4,5,6]. Benefited by their excellent optical and electrical properties, the devices based on these materials exhibit high detectivity and fast response for visible light. However, such materials are usually obtained by extremely complex approaches or using expensive equipment [7,8,9], which is a bottleneck on the way to their commercial application. Hence, seeking for more promising substitute materials to reduce the cost, and simplify the preparation process is very important.
Recently, hybrid halide perovskites (HHPs) materials have been one of the research hot spots in the field of photovoltaic devices [10,11,12,13,14,15]. In the last decade, the power conversion efficiencies of perovskite solar cells have been increased from 3.8% to exceed 23% [16,17,18,19,20,21,22,23,24,25,26,27], owing to its remarkable optoelectronic properties, such as the merits of the optimum bandgap, high absorption coefficient, and superior ambipolar carrier transport ability [28,29,30,31]. In addition, low-cost and simple solution process preparation also makes perovskites have great potential in the research of photodetectors. However, in spite of the photovoltaic devices based on HHPs have made rapid and impressive progress, they still suffer from poor stability [32, 33]. Compared with HHPs, inorganic cesium lead halide perovskites (IHPs) exhibit better stability in the air, indicating that IHPs is an ideal candidate for photodetectors [34, 35]. Although, CsPbI3 is unstable at high temperature (above 300 °C), which can be improved by substituting the Br− moiety for I− [36,37,38,39,40,41]. Therefore, CsPbI3-xBrx is very suitable for designing high-performance photodetectors.
In this work, we prepared CsPbI3-xBrx (x = 1, 2) films for flexible perovskite photodetectors (PDs). The flexible perovskite PDs based on CsPbI3-xBrx exhibited fast response speed (90 μs/110 μs for CsPbI2Br PDs and 100 μs/140 μs for CsPbIBr2 PDs), a high on/off ratio (104), and a high detectivity (1012 Jones) under 520 nm lamp with 10 mV bias. Meanwhile, it exhibited outstanding mechanical flexibility and environmental stability. After keeping the device for 30 days in ambient air at 35–45% relative humidity, the periodic I-t curves of the device are only slightly declined (~ 3%). In addition, after bending the flexible PDs for 100 times under the bending radius of 9.12 mm, the periodic I-t curves of the device showed negligible change (< 3% decrease). The results indicate the potential of CsPbI3-xBrx perovskites for flexible PDs.
Lead iodide (PbI2, 99.99%), lead bromide (PbBr2, 99.99%), barium iodide (CsI, 99.99%), and barium bromide (CsBr, 99.99%) were purchased from Xi’an Polymer Light Technology Corporation. Diethyl ether (DEE), acetone, absolute ethanol, N,N-dimethylformamide (DMF), and dimethylsulfoxide (DMSO) were provided by Sigma-Aldrich.
The perovskite solution was prepared as follows. The CsPbI2Br perovskite precursor solutions were prepared by mixing the 1 M (mol L−1) CsBr, 1 M PbBr2, 2 M CsI, and 2 M PbI2 in mixed anhydrous solvents of DMSO and DMF (9:1 in volume). The CsPbIBr2 perovskite precursor solutions were prepared by mixing the 2 M CsBr, 2 M PbBr2, 1 M CsI, and 1 M PbI2 in mixed anhydrous solvents of DMSO and DMF (9:1 in volume). Then, the mixed perovskite solutions were stirred at 75 °C more than 2 h. All solutions must be were prepared in a nitrogen glovebox.
Flexible substrates [polyimide (PI)] were cleaned consecutively with acetone, absolute ethanol, and deionized water for 15 min, respectively. And then the substrates were dried in an oven. Subsequently, interdigitated golden electrode (80 nm) was evaporated onto the flexible substrates by thermal evaporation. Before use, the patterned substrates were treated with UV-ozone for 20 min. Then the flexible substrates were transferred into glovebox for perovskite films deposition. The CsPbI3-xBrx films were prepared using anti-solvent (DEE) one-step spin-coating method. Eighty-microliter precursor solution was spin-coating at a speed of 2000 rpm for 60 s. Then, 0.5 mL diethyl ether was poured on the samples at 10 s before the end of the spinning-coating processes. Then, the samples were annealed at 65 °C for 5 min and 135 °C for 15 min.
Measurements and Characterizations
Scanning electron microscope (SEM) images were obtained by using field emission SEM (FEI- INSPECT F50, Holland). X-ray diffraction (XRD) was carried out using a Bede D1 system with Cu Kα radiation. The ultraviolet-visible (UV-vis) absorption spectrum was measured by an UV-vis spectrophotometer (Schimadzu UV-3101 PC). The current–voltage (I-V) curves were carried out by Keithley 2636 semiconductor parametric analyzer under the illumination of a LD light source. Photocurrent was measured with an oscilloscope (Agilent DOS5012A) and an optical chopper modulating the light illuminated on the device. All measurements were carried out under ambient conditions at room temperature.
Results and Discussion
Anti-solvents, which are often used in the preparation of perovskite films to obtain a high-quality surface morphology. Herein, we used one-step spin-coating method with anti-solvent (DEE) to improve the morphology of CsPbI3-xBrx films. Figure 1 exhibits the plan-view SEM images of CsPbI3-xBrx films with or without DEE treatment. As shown in Fig. 1a, b, the CsPbI2Br and CsPbIBr2 film without DEE-treatment possess enormous pinholes and small crystal grain size. In contrast, after DEE-treatment in the fabrication of perovskite, continuous film and larger grains are observed in the SEM images (Fig. 1c, d). The results of SEM images indicated that the morphology of the CsPbI3-xBrx films was significantly improved by the treatment of DEE. Therefore, in the subsequent work, the anti-solvent treatment process was adopted to prepare CsPbI3-xBrx films.
In order to examine the crystal structure of the prepared CsPbI3-xBrx films, XRD patterns were carried out. As shown in Fig. 2a, the red and the blue lines indicate the XRD patterns of CsPbIBr2 films and CsPbI2Br, respectively. It was clear to observe, in the red lines, the main peaks located at 14.75°, 20.94°, 29.96°, and 34.93°, which are assigned to the (100), (110), (200), and (210) facts of CsPbIBr2, respectively [41,42,43]. In the blue lines, we note two main peaks centered at 14.44° and 20.3° corresponding to the (100) and (200) planes of the pure CsPbI2Br α phase [44, 45]. In addition, to certify that the CsPbIBr2 and CsPbI2Br films were successfully prepared, UV-vis absorption curves and Tauc plots were measured (Fig. 2b–d). As shown in Fig. 2b, a small blue shift is visible in the absorption spectrum of the CsPbIBr2 film compared to the CsPbI2Br film, which attributed to the bandgap difference between CsPbI2Br and CsPbIBr2. To explore the optical bandgap of CsPbI3-xBrx film, we calculated the energy band (Eg) according to the reflection and transmission through the Tauc plots, as shown in Fig. 2c, d. It was observed from the Tauc plots that Eg of CsPbI2Br and CsPbIBr2 were 1.91 eV and 2.05 eV, respectively, which is consistent with the previous report [46,47,48,49,50]. The results indicated the CsPbI3-xBrx films were successfully fabricated.
After confirming the properties of the treated CsPbI3-xBrx films, we prepared the flexible PDs based on CsPbI3-xBrx films. In Fig. 3a, the flexible PDs with the device structure of PI/Au interdigitated electrodes/CsPbI3-xBrx are shown. When it is irradiated on the perovskite layer under a bias voltage, the charge carrier transport is formed in PDs, as shown in Fig. 3b. Finally, electrons (holes) are collected by electrodes and circulated through an external circuit to generate photocurrent. To characterize the performance of CsPbI3-xBrx PDs, we measured the photocurrent under 520 nm LD source at low bias voltages as shown in Fig. 3c, d. The result showed that the maximum photocurrent of CsPbI2Br PDs and CsPbIBr2 PDs were beyond 180 μA and 120 μA under the illumination intensity of 8.23 mW/cm2, respectively. Importantly, the photocurrent of the device was measured at a bias voltage of 10 mV. To evaluate the response speed of the device, we investigated the transient photocurrent of the device. As shown in Fig. 3c, d, the rise and decay time of CsPbI2Br PDs are extracted to be around 90 μs and 110 μs, respectively. The rise and decay time of CsPbIBr2 PDs were found to be about 100 μs and 140 μs, respectively. Compared to the same structural devices previously reported , the results manifested that the device based on DEE-treated CsPbI3-xBrx perovskite layer showed excellent performance.
To further investigate the photoelectrical characteristics of the PDs, the dark current and photo-current, responsivity, and detectivity were measured and plotted, as shown in Fig. 4. As showed in Fig. 4a, b, the dark current and photocurrent curves have approximate symmetry when the voltage was changed from − 5 to 5 V. This result indicated the formation of an ohmic contact between the metal and the perovskite layer. Owing to the contact barrier being very low for ohmic contact, carriers can be easily transferred under low bias. At low bias voltages, the CsPbI3-xBrx flexible PDs possess a high on/off ratio of approximately 104. Responsivity (R) and detectivity (D*) of the PDs were showed in Fig. 4c, d. The image illustrated that the R and D* had high values under weak light at low bias, especially below 1 mW, along with a high D* of 1012 Jones@10 mV bias. Zhang et al. reported a CsPbBr3-based flexible PDs with a D* of 1010 Jones under 2 V bias . Ding et al. reported a rigid PDs based on CsPbBr3 single crystals with a D* of 1011 Jones . Therefore, the CsPbI3-xBrx-based flexible PDs working under low bias voltages exhibit outstanding performances.
Environmental stability and mechanical flexibility are two important factors that influence the practical application of photodetectors based on perovskite. As described in Fig. 5, the environmental stability and mechanical flexibility of the PDs were tested by measuring the changes in periodic I-t curves of the device. It was clearly observed that the I-t curves of the device changed slightly (~ 3% decrease for CsPbI2Br PDs and ~ 3% decrease for CsPbIBr2 PDs). The changes of the devices’ currents could be ignored after being exposed for 30 days in ambient conditions at 35–45% relative humidity (Fig. 5a, b). As showed in Fig. 5c, d, compared with the initial periodic I-t curves, a negligible oscillation was observed (~ 2% decrease for CsPbI2Br PDs and ~ 3% decrease for CsPbIBr2 PDs) after bending the device for one hundred times under the bending radius of 9.12 mm. The results demonstrate that our device has a great stability as well as good mechanical flexibility.
In summary, we present the flexible photodetectors based on CsPbI3-xBrx (x = 1, 2) films which were treated with DEE in this work. The devices showed excellent performance, which were comparable to the same configuration devices. At a bias of 10 mV, the photodetectors showed a high on/off ratio of 104 under 520 nm illumination, fast response speed (90 μs/110 μs for CsPbI2Br PDs and 100 μs/140 μs for CsPbIBr2 PDs), and an excellent detectivity (1012 Jones). Furthermore, the flexible PDs exhibited outstanding environmental stability and mechanical flexibility. After storing the device for 30 days in air at 35–45% relative humidity, the I-t curves of the device are only slightly declined (~ 3%). In addition, performance of the PDs showed a negligible change after bending the flexible PD a hundred times with a bend radius of 9.12 mm. This work demonstrates the enormous potential of CsPbI3-xBrx perovskites in photoelectron detection and provides a promising approach to achieving high performance.
Availability of Data and Materials
The datasets used and/or analyzed during the current study are obtained from the corresponding author on reasonable request.
Hybrid halide perovskites
Inorganic cesium lead halide perovskites
Scanning electron microscope
Kojima A, Teshima K, Shirai Y et al (2009) Organometal halide perovskites as visible-light sensitizers for photovoltaic cells [J]. J Am Chem Soc 131(17):6050–6051
Wang L, Jie J, Shao Z et al (2015) MoS2/Si heterojunction with vertically standing layered structure for ultrafast, high-detectivity, self-driven visible–near infrared photodetectors. Adv Funct Mater 25(19):2910–2919
Zhang T, Liu B, Ahmad W et al (2017) Optical and electronic properties of femtosecond laser-induced sulfur-hyperdoped silicon N+/P photodiodes. Nanoscale Res Lett 12(1):522
Wang H, Kim DH (2017) Perovskite-based photodetectors: materials and devices. Chem Soc Rev 46(17):5204–5236
Chen S, Shen L, van Aken PA et al (2017) Dual-functionalized double carbon shells coated silicon nanoparticles for high performance lithium-ion batteries. Adv Mater 29(21):1605650
Fang Y, Dong Q, Shao Y et al (2015) Highly narrowband perovskite single-crystal photodetectors enabled by surface-charge recombination. Nat Photonics 9(10):679
Gong X, Tong M, Xia Y et al (2009) High-detectivity polymer photodetectors with spectral response from 300 nm to 1450 nm [J]. Science 325(5948):1665–1667
Baeg KJ, Binda M, Natali D et al (2013) Organic light detectors: photodiodes and phototransistors [J]. Adv Mater 25(31):4267–4295
Guo Y, Liu C, Tanaka H et al (2015) Air-stable and solution-processable perovskite photodetectors for solar-blind UV and visible light. J Phys Chem Lett 6(3):535–539
Zhang T, Wu J, Zhang P et al (2018) High speed and stable solution-processed triple cation perovskite photodetectors. Advanced Optical Materials 6(13):1701341
Wang Y, Zhang Y, Lu Y et al (2015) Hybrid graphene–perovskite phototransistors with ultrahigh responsivity and gain [J]. Advanced Optical Materials 3(10):1389–1396
Zhang T, Wang F, Zhang P et al (2019) Low-temperature processed inorganic perovskites for flexible detectors with a broadband photoresponse. Nanoscale 11(6):2871–2877
Qian C, Sun J, Kong LA et al (2017) High-performance organic heterojunction phototransistors based on highly ordered copper phthalocyanine/para-sexiphenyl thin films [J]. Adv Funct Mater 27(6):1604933
Yantara N, Bhaumik S, Yan F et al (2015) Inorganic halide perovskites for efficient light-emitting diodes. J Phys Chem Lett 6(21):4360–4364
Hu W, Huang W, Yang S et al (2017) High-performance flexible photodetectors based on high-quality perovskite thin films by a vapor–solution method [J]. Adv Mater 29(43):1703256
Lee MM, Teuscher J, Miyasaka T et al (2012) Efficient hybrid solar cells based on meso-superstructured organometal halide perovskites. Science 338(6107):643–647
Li S, Zhang P, Chen H et al (2017) Mesoporous PbI2 assisted growth of large perovskite grains for efficient perovskite solar cells based on ZnO nanorods [J]. J Power Sources 342:990–997
Burschka J, Pellet N, Moon SJ et al (2013) Sequential deposition as a route to high-performance perovskite-sensitized solar cells [J]. Nature 499(7458):316
Zhang P, Wu J, Zhang T et al (2018) Perovskite solar cells with ZnO electron-transporting materials. Adv Mater 30(3):1703737
Yang WS, Park BW, Jung EH et al (2017) Iodide management in formamidinium-lead-halide–based perovskite layers for efficient solar cells. Science 356(6345):1376–1379
Cai B, Xing Y, Yang Z et al (2013) High performance hybrid solar cells sensitized by organolead halide perovskites. Energy Environ Sci 6(5):1480–1485
Li S, Zhang P, Wang Y et al (2017) Interface engineering of high efficiency perovskite solar cells based on ZnO nanorods using atomic layer deposition. Nano Res 10(3):1092–1103
Chen Y, Yang Z, Wang S et al (2018) Design of an inorganic mesoporous hole-transporting layer for highly efficient and stable inverted perovskite solar cells. Adv Mater 30(52):1805660
Ji L, Zhang X, Zhang T et al (2019) Band alignment of Pb–Sn mixed triple cation perovskites for inverted solar cells with negligible hysteresis. J Mater Chem A 7(15):9154–9162
Wang P, Wu Y, Cai B, Ma Q, Zheng X, Zhang WH (2019). Solution‐Processable Perovskite Solar Cells toward Commercialization: Progress and Challenges. Adv Funct Mater. p. 1807661.
Wang F, Zhang T, Wang Y et al (2019) Steering the crystallization of perovskites for high-performance solar cells in ambient air. J Mater Chem A 7(19):12166–12175
Jeon NJ, Na H, Jung EH et al (2018) A fluorene-terminated hole-transporting material for highly efficient and stable perovskite solar cells [J]. Nat Energy 3(8):682
Leijtens T, Stranks SD, Eperon GE et al (2014) Electronic properties of meso-superstructured and planar organometal halide perovskite films: charge trapping, photodoping, and carrier mobility. ACS Nano 8(7):7147–7155
Gu X, Wang Y, Zhang T et al (2017) Enhanced electronic transport in Fe 3+-doped TiO2 for high efficiency perovskite solar cells [J]. J Mater Chem C 5(41):10754–10760
Saidaminov MI, Haque MA, Almutlaq J et al (2017) Inorganic lead halide perovskite single crystals: phase-selective low-temperature growth, carrier transport properties, and self-powered photodetection. Advanced Optical Materials 5(2):1600704
Liu D, Li S, Zhang P et al (2017) Efficient planar heterojunction perovskite solar cells with Li-doped compact TiO2 layer. Nano Energy 31:462–468
Tong X, Lin F, Wu J et al (2016) High performance perovskite solar cells. Advanced Science 3(5):1500201
Zhao Y, Zhu K (2016) Organic–inorganic hybrid lead halide perovskites for optoelectronic and electronic applications. Chem Soc Rev 45(3):655–689
Zhang J, Wang Q, Zhang X et al (2017) High-performance transparent ultraviolet photodetectors based on inorganic perovskite CsPbCl 3 nanocrystals. RSC Adv 7(58):36722–36727
Zhang X, Wang Q, Jin Z et al (2017) Stable ultra-fast broad-bandwidth photodetectors based on α-CsPbI 3 perovskite and NaYF 4: Yb, Er quantum dots. Nanoscale 9(19):6278–6285
Eperon GE, Paterno GM, Sutton RJ et al (2015) Inorganic caesium lead iodide perovskite solar cells. J Mater Chem A 3(39):19688–19695
Zhang Y, Liu Y, Li Y et al (2016) Perovskite CH 3 NH 3 Pb (BrxI1− x) 3 single crystals with controlled composition for fine-tuned bandgap towards optimized optoelectronic applications. J Mater Chem C 4(39):9172–9178
Yan L, Xue Q, Liu M et al (2018) Interface engineering for all-inorganic CsPbI2Br perovskite solar cells with efficiency over 14%. Adv Mater 30(33):1802509
Chen CY, Lin HY, Chiang KM et al (2017) All-vacuum-deposited stoichiometrically balanced inorganic cesium lead halide perovskite solar cells with stabilized efficiency exceeding 11%. Adv Mater 29(12):1605290
Wang P, Zhang X, Zhou Y et al (2018) Solvent-controlled growth of inorganic perovskite films in dry environment for efficient and stable solar cells. Nat Commun 9(1):2225
Sutton RJ, Eperon GE, Miranda L et al (2016) Bandgap-tunable cesium lead halide perovskites with high thermal stability for efficient solar cells. Adv Energy Mater 6(8):1502458
Liu C, Li W, Chen J et al (2017) Ultra-thin MoOx as cathode buffer layer for the improvement of all-inorganic CsPbIBr2 perovskite solar cells. Nano Energy 41:75–83
Ma Q, Huang S, Wen X et al (2016) Hole transport layer free inorganic CsPbIBr2 perovskite solar cell by dual source thermal evaporation. Adv Energy Mater 6(7):1502202
Beal RE, Slotcavage DJ, Leijtens T et al (2016) Cesium lead halide perovskites with improved stability for tandem solar cells. J Phys Chem Lett 7(5):746–751
Lau CFJ, Zhang M, Deng X et al (2017) Strontium-doped low-temperature-processed CsPbI2Br perovskite solar cells. ACS Energy Letters 2(10):2319–2325
Lau CFJ, Deng X, Ma Q et al (2016) CsPbIBr2 perovskite solar cell by spray-assisted deposition. ACS Energy Letters 1(3):573–577
Zeng Q, Zhang X, Liu C et al (2019) Inorganic CsPbI2Br perovskite solar cells: the progress and perspective. Solar RRL 3(1):1800239
Dong C, Han X, Zhao Y et al (2018) A green anti-solvent process for high performance carbon-based CsPbI2Br all-inorganic perovskite solar cell. Solar RRL 2(9):1800139
Yin G, Zhao H, Jiang H et al (2018) Precursor engineering for all-inorganic CsPbI2Br perovskite solar cells with 14.78% efficiency. Adv Funct Mater 28(39):1803269
Wang Y, Zhang T, Xu F et al (2018) A facile low temperature fabrication of high performance CsPbI2Br all-inorganic perovskite solar cells. Solar RRL 2(1):1700180
Ding J, Du S, Zuo Z et al (2017) High detectivity and rapid response in perovskite CsPbBr3 single-crystal photodetector. J Phys Chem C 121(9):4917–4923
This work was supported by the National Natural Science Foundation of China under Grant Nos. 61421002, 61874150 and 61574029.
National Natural Science Foundation of China: 61421002, 61874150, and 61574029.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Liu, Z., Li, H., Qin, C. et al. Solution-Processed Inorganic Perovskite Flexible Photodetectors with High Performance. Nanoscale Res Lett 14, 284 (2019). https://doi.org/10.1186/s11671-019-3120-x
- CsPbI3-xBrx-based flexible PDs
- Low bias voltage
- Environmental stability
- Mechanical flexibility